# 4860 Molenaar III

date post

10-Nov-2015Category

## Documents

view

25download

4

Embed Size (px)

description

### Transcript of 4860 Molenaar III

CT 4860 Structural Design of Pavements January 2009 Prof.dr.ir. A.A.A. Molenaar

PART III

Design of Flexible Pavements

2

Table of contents Preface 3 1. Introduction 4 2. Major defect types in flexible pavements 5 2.1 Cracking 6 2.2 Deformations 9 2.3 Desintegration and wear 11 3. Early design systems, the CBR method 11 4. AASHTO design method 14 5. Development of mechanistic empirical design methods 25 5.1 Introduction 25 5.2 Stresses in a homogeneous half space 27 5.3 Stresses in two layer systems 32 5.4 Stresses in three layer systems 41 5.5 Stresses due to horizontal loads 47 5.6 Stresses in multilayer systems, available computer programs 51 6. Axle loads, wheel loads and contact pressures 69 6.1 Axle loads 69 6.2 Wheel loads 74 6.3 Contact pressures 75 7. Climatic data 84 7.1 Introduction 84 7.2 Temperature 84 7.3 Moisture 89 8. Asphalt mixtures 94 8.1 Introduction 94 8.2 Mixture stiffness 94 8.3 Fatigue resistance 102 8.4 Resistance to permanent deformation 108 9. Granular materials 111 9.1 Introduction 111 9.2 Estimation of the resilient characteristics of sands and unbound materials 111 9.3 Estimation of the failure characteristics of unbound materials 121 9.4 Allowable stress and strain conditions in granular materials 124 10. Base courses showing self cementation 125 11. Cement and lime treated materials 131 11.1 Introduction 131 11.2 Lime treated soils 132 11.3 Cement treated materials 133 12. Subgrade soils 140 12.1 Introduction 140 12.2 Estimation of the subgrade modulus 140 12.3 Allowable subgrade strain 142 13. Special design considerations 143 13.1 Introduction 143 13.2 Edge effect 143 13.3 Reflective cracking 145 14. Design systems 150 14.1 Introduction 150 14.2 Shell pavement design software 150 14.3 ASCON design system 151 14.4 TRH4 155 References 163

3

Preface In these lecture notes the design of flexible pavements by means of mechanistic empirical methods is discussed. What do we mean by mechanistic empirical methods? By mechanistic we mean that the design methods are based on the analysis of stresses and strains in the pavement structure due to traffic loads or environmental effects using multi layer theory. In order to be able to make such analyses, assumptions need to be made on the behaviour of the material. We can e.g. assume that pavement materials behave linear elastic, isotropic and homogeneous. This however is a serious simplification of reality because most pavement materials exhibit a stress dependent, elasto-visco-plastic behaviour. In any case the calculated stresses and strains are then used as input in a transfer function (e.g. a fatigue relation) that allows us to calculate how many times a particular tensile strain can occur before failure occurs. This part of the design method is the empirical part. The reason for this is that although these transfer functions are usually based on extensive material testing in the laboratory, most of these tests give a specimen property rather then a material property. In other words: the material characteristic derived from the test result is dependent on the geometry of the test as well as the way in which the test was performed. Because of this and because the significant differences in stress conditions as used in the laboratory and those that occur in practice, as well as the differences in damage initiation and progression between laboratory specimens and real pavements, the transfer functions as determined in the laboratory cannot be applied directly to calculate the number of load repetitions to failure for a specific pavement. This implies that shift factors need to be applied in order to be able to use the laboratory determined transfer functions for practical purposes. These shift factors often are of significant magnitude and are commonly based on matching predicted behavior to observed behavior. This makes them dependent on the local conditions and type of pavement structure involved and empirical knowledge is needed to derive and use these shift factors successfully. All this explains why the current design methods are classified as mechanistic empirical. In these lecture notes we will concentrate on the use of linear elastic multi layer theory for the calculation of stresses and strains in pavement structures. It will be assumed that the materials are isotropic, homogeneous and linear elastic. Ample attention however will also be paid to how the stress dependent, non linear behaviour of unbound materials can be taken into account. Furthermore the collection of input needed to make a mechanistic empirical based design will be discussed extensively. Great care has been given to the preparation of these notes; some errors however can never be avoided. It is therefore greatly appreciated if you inform the authors about any typing errors you may find. Prof. dr. ir. A.A.A. Molenaar [email protected]

4

1. Introduction

These lecture notes are dealing with the design of flexible pavements. Before we start with start with a discussion on stress and strain analyses in such pavements, we better ask ourselves what is a flexible pavement or what do we define as being a flexible pavement. In these notes all pavements which are not considered to be a cement concrete pavement or a concrete block (small element) pavement are considered to be a flexible pavement. This implies that also pavements with a relatively stiff cement treated subbase or base are classified as a flexible pavement. Some examples of what is considered to be a flexible pavement are given in figure 1.

Figure 1: Different types of flexible pavement structures. In the South African structures, the bearing capacity of the pavement is provided by the unbound base and subbase (structure I) or by the unbound base and cement treated subbase (structure II). The asphalt top layer provides a smooth riding surface and provides skid resistance. These structures have been successfully used in South Africa for moderately (structure I) and heavily loaded (structure II) roads. The secrets of the success of these pavements are the high quality,

I 50 mm asphalt concrete top layer; 150 mm unbound base; 150 mm un-bound subbase; subgrade SOUTH AFRICA

II 50 mm asphalt concrete top layer; 150 mm unbound base; 150 mm cement trea-ted subbase; subgrade SOUTH AFRICA

III 50 mm porous asphalt con-crete; 200 mm asphalt con-crete; 300 mm unbound base of recycled mate-rial; subgrade NETHERLANDS

IV 200 mm polymer modified asphalt concrete; 600 mm lean concrete base; subgrade SCHIPHOL AIRPORT AMSTERDAM

5

abundantly available, crushed materials used for the base and subbase and the high levels of compaction achieved. Furthermore the minimum CBR required for the subgrade is 15%. When that is not reached, improvement of the subgrade should take place. The cement treated subbase as used in structure II not only provides a good working platform for the construction and compaction of the unbound base but also influences the stress conditions in the pavement such that relatively high horizontal confining stresses develop in the unbound base. As we know from the lectures on unbound materials (CT4850), unbound materials become stiffer and stronger when the degree of confinement increases. Structure III is an example of a highway pavement structure in the Netherlands. One will observe immediately the striking difference between structure II which is used for heavily loaded pavements in South Africa and structure III that is used in the Netherlands for these purposes. The reasons for these differences are quite simple being that the conditions in the Netherlands are completely different. There are e.g. no quarries in the Netherlands that can provide good quality crushed materials; these have to be imported from other countries. However, limitations in space and strict environmental requirements require to recycle materials as much as possible. Since it has been shown that good quality base courses can be built of mixtures of crushed concrete and crushed masonry, extensive use is made of unbound base courses made of these recycled materials. A porous asphalt concrete top layer is used (void content > 20%) for noise reducing purposes. The thickness of the entire pavement structure is quite significant because the bearing capacity of the subgrade is quite often not more than 10%. The main reason for the large thickness however is that the road authorities dont want to have pavement maintenance because of lack of bearing capacity. Such maintenance activities involve major reconstruction which cause, given the very high traffic intensities, great hinder to the road user which is not considered to be acceptable. For that reason pavement structures are built such that maintenance is restricted to repair or replacement of the top layer (porous asphalt concrete). With respect to compaction of the unbound base it should be noted that it would be very hard to achieve the same results in the Netherlands as in South Africa. In South Africa the excellent compaction is achieved by soaking the base material and using a high compaction effort. The excessive amount of water used easily disappears because of the high evaporation rates. The recycled materials used for base courses in the Netherlands contain a significant amount of soft material (masonry) which is likely to crush if the compaction effort is too heavy. Furthermore the excessive amount of water used for compaction will not disappear easily because of the much lower evaporation rates. Using the South African way of compacting granular base and subbase courses in the Netherlands will therefore not lead to similar good results. Structure IV is the structure used for the runways and taxiways of Amsterdams Schiphol Airport. The airport is situated in a polder with poor subgrade conditions (CBR 2%). Combined with the airports philosophy to maximize the use of the runway and taxiway system and minimize the need for maintenance, this results in rather thick pavement structures. A total thickness of 200 mm polymer modified asphalt concrete is used to reduce the risk for reflective cracking. For that reason the lean concrete base is also pre-cracked. From the discussion given above it becomes clear that the type of pavement structure to be selected depends on the available materials, climatic conditions, maintenance philosophy etc. From the examples given above it also becomes clear that one has to be careful in just copying designs which seem to be effective and successful in other countries. One always has to consider the local conditions which influence the choice of a particular pavement type.

2. Major defect types in flexible pavements Pavements are designed such that they provide a safe and comfortable driving surface to the public. Of course they should be designed and constructed in such a way that they provide this surface for a long period of time at the lowest possible costs. This implies that the thickness

6

design and the material selection should be such that some major defect types are under control meaning that they dont appear too early and that they can be repaired easily if they appear. Major defect types that can be observed on flexible pavements are:

- cracking, - deformations, - disintegration and wear.

A short description of these defect types and their causes is given hereafter. Later in these notes it will be described how these defect types are taken care of in pavement design.

2.1 Cracking Cracks in pavements occur because of different reasons. They might be traffic load associated or might develop because of thermal movements or some other reason. Figure 2 e.g. shows a combination of wheel track alligator cracking and longitudinal cracking. These cracks are wheel load associated. Figure 2: Longitudinal and alligator cracking in the Wheel path.

Please note that the cracks only appear in the right hand wheel track close to the edge of the pavement. This is an indication that the cracks are most probably due to edge load conditions resulting in higher stresses in the wheel track near the pavement edge than those that occur in the wheel track close to the center line. Because of this specific loading condition, cracks might have been initiated at the top of the pavement. Figure 3 is a picture of a cracked surface of a rather narrow pavement. If vehicles have to pass each other, the outer wheels have to travel through the verge. From the edge damage that is observed one can conclude that this is regularly the case. The base material which is visible in the verge seems to be a stiff and hard material. This is an indication that some kind of slag that shows self cementing properties was used as base material. Further indications of the fact that such a base material has been used can be found from the fact that the pavement surface is smooth; no rutting is observed. The extensive cracking of the pavement surface might be a combination of shrinkage cracks that have developed in the base. It is however also very well possible that the adhesion between the asphalt layer and the base is rather poor. If this is the case then high tensile strains will develop at the bottom of the asphalt layer causing this layer to crack.

7

Figure 3: Cracking observed on a narrow polder road in the Netherlands.

Figure 4: Low temperature cracking observed on a highway in Minnesota.

Figure 4 is a typical example of low temperature cracking. In areas with cold winters, this type of cracking is quite often the dominating cracking type. Due to the very cold weather, the asphalt concrete wants to shrink. In principle this is not possible and tensile stresses develop as a result of the drop in temperature. The magnitude of the tensile stress depends on the rate of cooling and the type of asphalt mixture; especially the rheological properties of the bituminous binder are of importance. If the tensile stresses are becoming too high, the pavement will crack at its weakest point. Further cooling down of the pavement results in additional cracking and existing cracks will open. It is obvious that crack spacing and crack width are interrelated. A large crack spacing results in wide cracks and vice versa. Low temperature cracking can be the result of a single cooling down cycle but also can be the result of repeated cooling down cyclces (low temperature fatigue). Figure 5 is an example of temperature related block cracking. The pavement of course not only shrinks in the longitudinal direction but also in the transversal direction. In that case the friction between the asphalt layer and the base is of importance. If that is high, high tensile stresses might occur in the transversal direction causing longitudinal cracks. Combined with the crack pattern shown in figure 4, this results in block cracking.

8

Figure 5: Low temperature associated block cracking observed on a highway in Minnesota. A type of cracking that has many similarities with low temperature cracking is reflective cracking. In that particular case, a crack or joint in the layer underneath the asphalt layer tends to propagate through the asphalt layer. The problem often occurs in pavements with a cement treated base or overlaid jointed concrete pavements (figure 6). Reflective cracking can even occur in new pavements when the cemented base shrinks due to hardening. Shrinkages cracks that develop in the base can easily reflect through the asphalt top layer especially if this layer is thin. If however the cement treated base is pre-cracked or if shrinkage joints have been made, the problem of reflective cracking can be minimized.

In these lecture notes we will concentrate on traffic induced cracking as well as reflective cracking. Low temperature is not considered because it is not really an issue in the Netherlands with its moderate climate. Of course cracks can develop for many other reasons then traffic and environmental effects. One example of such another reason is given in figure 7 which shows severe cracking in the emergency lane due to the widening of the embankment next to that lane. Due to the widening, excessive shear stresses developed in the existing embankment resulting in the development of a shear plane leading to severe longitudinal cracking not only in the emergency lane but also in the slow lane (this lane is already repaired as the picture shows). The problem was aggravated by

As mentioned before, low temperature cracking can be the major cause of main-tenance and traffic associated cracking is only of secondary importance in such cases. However, when heavy wheel loads are passing a crack like the one shown in figure 4, high tensile stresses will develop at the crack edge simply because of the fact that there is no load transfer. This problem might increase during the spring when moisture enters the crack and weakens the supporting layers. All this means that although traffic associated cracking is not the main problem, traffic can cause accelerated damage development near cracks.

Figure 6: Example of reflective cracking in an overlaid jointed concrete pavement.

9

Figure 7: Severe longitudinal cracking due to shear failure in the existing embankment as a

result of widening the road (extended embankment is on the right had side).

2.2 Deformations Deformations in pavements can be divided in longitudinal and transverse deformations. Longitudinal deformations can further by divided in short, medium and long wave deformations. Short wave deformations are of the order of a few centimeters and are mainly caused by surface irregularities such as raveling (this will be discussed later). Medium wave deformations are in the order of a few decimeters and usually are caused by imperfections in the pavement structure itself. Long wave deformations are in the order of meters and are caused by settlements, swelling soils, frost heave etc. Although they cause major annoyance, long wave deformations are, because of their origin, outside the scope of these lecture notes.

Figure 8: Roughness due to severe cracking.

the fact that a significant height difference occurred across the longitudinal crack resulting in very dangerous driving conditions for motor cyclists. This type of cracking is clearly due to a soil mechanics problem and therefore is beyond the scope of these lecture notes.

Therefore we will restrict ourselves to short and medium wave length longitudinal deformations, also called unevenness or roughness. Figure 8 shows a severely cracked farm to mar-ket road in Ohio. Due to the extensive amount of cracking, the pavement has become rather rough. It is quite clear from the picture that cracking has not only resulted in longitudinal but also transverse deformations. It is a typical example of medium wavelength roughness. Figure 9 shows a pavement in Zimbabwe. Lack of maintenance has resulted in potholes which ob-viously result in a large decrease of driving com-fort. Even dangerous situations might occur when driving at night. The reason for the pot-holes is that pavement has cracked severely, comparable to a condition shown in figure 8, and at given moment small pieces of the surface layer have been driven out. Erosion of the pot-holes due to rain and wind results in depressions of significant size and depth. Figure 9: Roughness due to potholes as a result

of severe cracking.

10

Figure 10: Longitudinal deformations due to settlements.

Figure 11: Rutting in an asphalt pavement.

Figure 12: Unevenness due to buckling of the base made of blast furnace slag.

Figure 10 was taken on a provincial road close to the Delft University in the Netherlands. The long wave longitudinal unevenness that can be observed is clearly the result of settlements. Please note that the settlements also have caused deforma-tions in the transverse direction. Next to longitudinal deformations, transver-sal deformations can occur. These can be the result of movement of the subsoil (settle-ments, swell, frost heave), but they also might be the result of traffic. The best known transversal deformation type due to traffic is rutting or permanent deformation that occurs in the wheel paths. A typical example of rutting is shown in figure 11. Rutting can develop in the asphalt layer(s) or in the unbound base, subbase or subgrade. Rutting can be the result of a densification process or as a result of shear failure. The rutting shown in figure 11 is clearly caused by shear failure in the asphalt layer. Shear failure can be recognized by the ridges that have de-veloped next to the depression. Furthermore one can state that the narrower the depress-sion the higher the layer is located in the structure where the shear failure has deve-loped. The same is true for corrugations or washboard formation that is quite often ob-served near traffic lights or on unsurfaced roads. Figure 12 shows a type of longitudinal un-evenness that is quite often observed on pavements with a base course made of blast furnace slags. Because of the chemical reactions that take place, the material wants to expand resulting into compressive stresses that at a given moment become higher than the compressive strength of the material. Buckling of the base course is then the result leading to ridges which negatively influence driving comfort and which might have a negative effect on traffic safety because of loss of cargo from trucks.

11

2.3 Desintegration and wear Raveling, bleeding and pothole formation can be rated as signs of disintegration and wear. Pothole formation has already been discussed in the previous section so we will concentrate ourselves in this section on raveling and bleeding. Bleeding is a defect type that can be recognized as black, fatty looking spots on the pavement surface. It is an indication of overfilling of the voids in the aggregate skeleton with bituminous mortar. It is an indication that the mixture is not well designed. Due to the high bitumen content, the mixture suffers probably from lack of stability at higher temperatures and high traffic loads might squeeze out the bituminous mortar. Another reason might be that because of the low void content, there is not enough space for the bituminous mortar when it expands with increasing temperatures. In any case, the result is the same being a black, shiny surface with hardly any macro or micro texture and thus a low skid resistance. Raveling is the loss of aggregate from the surface layer. It can occur on any type of asphalt mixture but especially open graded mixtures like porous asphalt concrete (void content > 20%) are sensitive for this damage type (figure 13). Raveling develops because of cohesive failure in the bituminous mortar or adhesive failure in the interface between aggregate and bituminous mortar.

Raveling provides a rough pavement surface resulting in an increased noise level. Furthermore the loose aggregate particles might result in windscreen damage. If raveling occurs on pavements with a thin asphalt surfacing, like the one shown in figure 9, it might be the first indication of pothole formation.

3. Early design systems, the CBR method Until now we have discussed damage types that can occur on flexible pavements. Before we start discussing the mechanistic empirical design systems that are developed, some information on the early design systems is given. Some knowledge on these systems is necessary because they are still used in several parts of the world and because it gives an understanding on how and why design systems developed to the mechanistic empirical systems used nowadays. Figure 14 is an

Figure 13: Raveling in porous asphalt concrete.

Note: some aggregate particles are naked without any mortar bonded to the aggregate surface.

12

example of the problems one encountered in the early years of motorization. In those days most roads were earth or gravel roads and the strength of the pavement solely depended on the shear strength of the materials used.

One has to realize that nowadays about 65% of the global road network still consists of earth and gravel roads. Problems as shown in figure 14 therefore still quite often occur as is shown in figure 15.

In both cases it is clear that the stresses induced in the pavement are higher than the allowable ones resulting in shear failure of the pavement surface and resulting in the fact that in both cases the vehicle got stuck in the mud. The question now is why a light vehicle, such as shown in figure 14, suffered from the same problems as the heavy vehicle shown in figure 15. This has to do with the fact that the contact pressures caused by the light vehicle shown in figure 14 are of the same order of magnitude as the contact pressures caused by the heavy vehicle shown in figure 15. The lesson we learn from this is that it is not really the weight of the vehicle that is of importance or the number of axles but the contact pressure distribution under the tires. This distribution not only depends on the wheel load but also on the area over which the wheel load is distributed. This depends to a very large extent on the tire pressure. In the old days, solid tires were initially used and when pneumatic tires were introduced, high tire pressures had to be used because of the size of the tire (see figure 14). This resulted in small contact areas and high contact pressures (as comparison: the contact pressure under the tire of a race bicycle is high because these tires are inflated to 700 kPa pressure; the contact area is also small). All this means that the contact pressure due to the vehicle shown in figure 14 could very well be the same as the contact pressure due to the vehicle shown in figure 15. Therefore similar types of surface defects can be expected.

Figure 14: Pavement problem in the early years of motorization.

Figure 15: Timber truck completely stuck on an earth road due to too high contact pressures and a too low shear resistance of the pavement material.

13

The other reason why both vehicles run into problems is the lack of bearing capacity of the pavement material. On both pictures we notice an excessive amount of water and from our lectures in soil mechanics we know that an excessive amount of water results in a low shear resistance especially in case of soils which contain a high amount of fine grained materials. We all know that the undrained shear strength of a saturated clay or silt is very low. In that case the cohesion is low and the angle of internal friction is about zero. From this example it is clear that precise knowledge on the pressures applied to the pavement and the strength of the materials used is essential in order to be able to design pavements that can sustain millions of load repetitions. The early design systems were, not surprisingly, based on determining the required thickness of good quality layers on top of the subgrade to prevent shear failure to occur in the subgrade. Of course the required thickness was dependent on the shear resistance of the subgrade and the amount of traffic. Furthermore the quality of the covering layers had to be such that shear failure didnt occur in these layers. This was the basis for the CBR thickness design method which is schematically shown in figure 16. In the CBR design charts, the traffic load was characterized by means of a number of commercial vehicles per day and the shear resistance of the materials was characterized by means of their CBR value. The charts were used in the following way. First of all the number of commercial vehicles had to be determined. When this number was known, the appropriate curve had to be selected. Next the CBR value of the subgrade needed to be determined and the required layer thickness on top of the subgrade could be estimated by means of figure 16; this will be illustrated by means of an example. If e.g. the subgrade CBR is equal to %, then the total thickness on top of the subgrade of a better quality material should be H1. If the CBR of the base material (for reasons of simplicity no subbase is applied in this case) is equal to , then the thickness of a better quality material (better than the base material) on top of the base should be H2. In most cases such a material would be asphalt concrete so H2 would be equal to the required asphalt thickness. The thickness of the base is then H1 H2.

Figure 16: Principle of the CBR design charts.

Increasing amount of traffic

H1

H2 log CBRsubgrade

Thickness

14

The minimum asphalt thickness to be applied was 50 mm. The CBR values of the unbound materials used in the pavement structure is determined by means of the CBR test which is schematically shown in figure 17. Although the test has been described in detail in the part I of the lecture notes CT4850, a summary of the basics of the test will be given here. In the CBR test a plunger is pushed into the soil sample with a specific displacement rate and the load that is needed to obtain that displacement rate is monitored. The load displacement curve that is obtained in this way is compared to the load displacement curve of a reference material and the CBR is calculated as shown in figure 18. The CBR design method results in thin asphalt layers which are mainly needed to provide a smooth driving surface and sufficient skid resistance.

4. AASHTO design method In the late 1950s, it was understood that, with the rapid increase in number and weight of the vehicles, these simple systems were not good enough anymore for the design of pavements and a strong need for improved methods developed. For that reason the American State Highway and Transportation Officials (AASHTO) launched a large research program that had to result in a better understanding of pavement performance in general and in a system that would allow durable and economical feasible pavement structures to be designed. For that reason a number of flexible and rigid pavement test sections were built which were subjected to a variety of traffic loads. This test is known as the AASHO Road Test, the results of which, e.g. the load equivalency concept, are still used today.

Figure 17: Principle of the CBR test.

15

Figure 18: Assessment of the CBR value.

It is beyond the scope of these lecture notes to discuss the Road Test in detail. The interested reader is referred to reference [1]. We will limit ourselves to a short description of the Interim Design Guide published in the early 1980s [2]. It is important to understand the principles of this guide since it is still being used in many places all around the world. One of the most important concepts that was developed during the test was the present serviceability index (PSI). This index is a number that reflects the service that is given by the pavement to the road user. The index was developed by correlating the physical condition of the various test sections in terms of the amount of cracking, rutting and unevenness to the ratings given by a panel of road users to the service provided by the pavement to the user. This latter rating was a number ranging from 5, being very good, to 0, being very poor. For main roads a PSI level of 2.5 was considered to be minimum acceptable level. The PSI is calculated as follows: PSI = 5.03 1.91 log ( 1 + SV ) 1.38 RD2 - 0.01 ( C + P ) Where: PSI = serviceability index, SV = slope variance, a measure of the unevenness of the pavement surface, C + P = percentage of cracked and patched pavement surface, RD = rut depth. As one could expect, the unevenness of the pavement has a significant effect on the PSI value; it dominates all the other factors. Detailed analyses of the data however showed that the amount of cracking and the slope variance correlate well with each other. The pavement design method that was developed using the results of the AASHO Road Test involves the calculation of the so called structural number in relation to the allowable drop in PSI and the number of load repetitions after which this drop in PSI is allowed to occur. The structural number SN is calculated using: SN = a1D1 + a2D2 + a3D3

reference material

material as tested

load

Fr

Fm

CBR = Fm / Fr * 100%

displacement

0.1 inch

16

Where: ai = structural coefficient of layer i [-], Di = thickness of layer i [inch], i = 1 is the asphalt layer, 2 = base, 3 = subbase. Other factors that are taken into account are the effective resilient modulus of the subgrade. Furthermore the method allows to design pavements with a certain level of reliability. Also the variation that occurs in the prediction of the occurring number of load repetitions as well as the variation that occurs in the layer thickness, structural layer coefficient and subgrade modulus can be taken into account by means of the overall standard deviation. The design chart is shown in figure 19. The subgrade modulus might vary during the year due to seasonal variations. One therefore has to determine the effective roadbed resilient modulus which is determined using the chart given in figure 20. Figure 20 is used as follows. One first determines the modulus which is to be used in a particular month (please note that it also possible to define the subgrade modulus each half month). Then the relative damage is determined using the scale at the right hand part of the figure. Next to that the sum is determined of the damage factors and divided by 12 (or 24 if the damage factor is defined per half month). This value is then used to determine the effective roadbed or subgrade modulus. An example of how to use the chart is given in table 1. Month Roadbed soil modulus [psi] Relative damage uf January 20,000 0.01 February 20,000 0.01 March 2,500 1.51 April 4,000 0.51 May 4,000 0.51 June 7,000 0.13 July 7,000 0.13 August 7,000 0.13 September 7,000 0.13 October 7,000 0.13 November 4,000 0.51 December 20,000 0.01 Average uf 3.72 / 12 = 0.31

Table 1: Calculation of the mean relative damage factor for the estimation of the effective subgrade modulus.

Since the mean relative damage factor = 0.31, we determine from figure 20 that the mean effective roadbed (or subgrade) modulus is 5,000 psi.

17

Figure 19: AASHTO design chart for flexible pavements based on using mean values for each input.

18

Figure 20: Chart to determine the effective roadbed (subgrade) modulus.

19

Charts to determine the structural layer coefficients for asphalt concrete, base and subbase are given in figures 21, 22 and 23.

The charts given in figures 22 and 23 are based on the following equations: For the base: a2 = 0.249 log EBS - 0.977 For the subbase: a3 = 0.227 log ESB 0.839 Both the resilient modulus of the base, EBS, and the subbase, ESB, are stress dependent following E = k1 k2 Where: E = modulus [psi],

= sum of the principal stresses [psi] (see table 2). k1, k2 = material constants (see table 3).

The sum of the principal stresses in the base and subbase depends of course on the thickness and stiffness of the layers placed on top of them as well as on the magnitude of the load. Suggested values for are presented in table 2. As one will notice from table 3, the material constants k1 and k2 are dependent on the moisture condition of the material (dry, damp, wet) as well as the quality of the material (indicated by the range in values.

Figure 21: Chart for determining the structural layer coefficient for asphalt; please note that the asphalt modulus is at 68 0F (20 0C).

20

Table 3: Values for k1 and k2 for base and subbase materials.

Also charts have been provided for cement treated bases and bituminous treated base courses. These charts are shown in figures 24 and 25. The traffic load is expressed as number of equivalent 18 kip (82 kN) single axles. To get this number the following equation is used. Neq = i=1i=n (Li / 82)4 Where: Neq = number of equivalent 18 kip (82 kN) single axles, n = number of axle load classes,

Li = axle load of axle load class i.

The reliability level to be used depends on the importance of the road. Freeways and very important highways are to be designed with a high level of reliability (90% and higher) because of the fact that traffic delays due to maintenance because of premature failure is not considered acceptable. Roads of minor importance can be designed with a much lower reliability level. Low volume roads e.g. can be designed with a reliability level of 60 70%. The overall standard deviation is much more difficult to estimate. It appeared that this value was 0.45 for the asphalt pavements of the AASHO Road Test. Because production and laying techniques have significantly be improved since then, a lower value could be adopted. Since it is difficult to estimate a proper value, use of the 0.45 value is still suggested.

Roadbed resilient modulus [psi] Asphalt concrete thickness [inch] 3000 7500 15000 < 2 20 25 30 2 4 10 15 20 4 6 5 10 15 > 6 5 5 5

Table 2: Estimated values for in the base and subbase.

21

Figure 22: Chart to estimate the structural layer coefficient for granular base courses.

22

Figure 23: Chart to estimate the structural layer coefficient for granular subbases.

23

Figure 24: Chart to estimate the structural layer coefficient of cement treated base layers.

24

Drainage is a very important feature of pavement structures. Insufficient drainage might result in moisture conditions close to saturation. As we have seen in table 3, such conditions result in significant lower values for k1 implying that the modulus of the unbound base and subbase can be 3 times lower in wet conditions than when they are dry. In order to be able to take care for improper drainage, it is suggested to multiply the structural layer coefficients with a drainage factor (mi) following: SN = a1D1 + m2a2D2 + m3a3D3 Recommended m values are given in table 4. It should be noted that the selection of the actual layer thicknesses has to follow a certain procedure. First of all one should determine the SN of the entire structure. Following the example in figure 20, we determine that the required SN = 5. Then we determine the required SN1 on top of the base. Assuming a modulus of 30000 psi for the base (a2 = 0.14) we determine that SN1 = 2.6 and we determine the required asphalt thickness (assuming a1 = 0.4) as D1 = SN1 / a1 = 2.6 / 0.4 = 6.5 inch. If we assume that the modulus of the subbase is 15000 psi (a3 = 0.11), we

Figure 25: Chart to estimate the structural layer coefficient for bituminous treated base courses.

25

Table 4: Drainage factor m.

5. Development of mechanistic empirical design methods 5.1 Introduction Although the AASHTO design method was a major step forward it still had the drawback of being highly empirical. The method in fact is nothing less than a set of regression equations which are valid for the specific conditions (climate, traffic, materials etc.) of the Road Test. This implies that it is a bit risky to use the method in tropical countries where the conditions are completely different. Fortunately, road constructions are forgiving structures implying that the method at least results in an initial design that can be refined to meet local conditions. The fact that the AASHTO method cannot be directly used for conditions for which it hasnt been developed became very apparent when attempts were made to use it in developing countries. The main problem was the PSI concept; it appeared e.g. that a pavement in the developed world with a low PSI implying that immediate maintenance was needed, was still a pavement with an acceptable quality in developing countries. This clearly indicated the need to have performance criteria and design methods that fit the needs and circumstances in developing countries. All this resulted in the development of the Highway Design Model [3], a design system that is fully suited for those conditions. It is however beyond the scope of these lecture notes to discuss this model in detail. Another problem with the Guide is that it gives no information why materials and structures behave like they do. Furthermore the Guide provides no information with respect to maintenance that is needed from a preservation point of view. The PSI value e.g. is strongly dependent on pavement roughness and damage types like cracking and rutting dont seem to have a large influence on the PSI. However control of cracking and rutting is important from a preservation point of view and in order to be able to make estimates on such maintenance needs, knowledge on stresses and strains and strength of materials is essential. Furthermore, if such information is not available, then it is almost impossible to evaluate the potential benefits of new types of materials and structures with which no experience has been obtained yet.

determine in the same way the required thickness on top of the subbase as SN2 = 3.4 The required base thickness is D2 = (SN2 SN1) / a2 = (3.4 2.6) / 0.14 = 5.8 inch. Furthermore we calculate the thickness of the subbase as D3 = (SN3 SN2) / a3 = (5 3.4) / 0.11 = 14.6 inch.

26

Given these drawbacks, one realized immediately after the Road Test that mechanistic based design tools were needed to support the AASHTO Guide designs. For that reason, much work has been done in the 1960s on the analysis of stresses and strains in layered pavement systems [6, 7, 8, 9] and on the characterization of the stiffness, fatigue and permanent deformation characteristics of bound and unbound pavement materials. The work done on the analysis of stresses and strains in pavements is all based on early developments by Boussinesq [4] and Burmister [5]. References [10, 11 and 12] are excellent sources with respect to research on pavement modeling and material characterization done in those days and should be on the reading list of any student in pavement engineering. It is remarkable to see that much of the material presented then still is of high value today. Since then, much progress has been made and the reader is referred e.g. to the proceedings of the conferences organized by the International Society of Asphalt Pavements, the proceedings of the Association of Asphalt Pavement Technologists, the Research Records of the Transportation Research Board, the proceedings of RILEM conferences on asphalt materials, the proceedings of the International Conferences on the Bearing Capacity of Roads and Airfields and those of many other international conferences to get informed about these developments. Given the possibilities we have nowadays with respect to material testing, characterization and modeling, it is possible to model pavements structures as accurate as possible using non linear elasto-visco-plastic models and using advanced finite element techniques that allow damage initiation and progression to be taken into account as well as the effects of stress re-distribution as a result of that. Also such methods allow the effects of joints, cracks and other geometry related issues to be taken into account. Furthermore these methods also allow to analyze the effects of moving loads which implies that inertia and damping effects can be taken into account. The question however is to what extent such advanced methods should be used for solving day to day problems. This is a relevant question because advanced pavement design methods involve advanced testing and analyses techniques which require specific hardware and skills. Furthermore pavement design is to some extent still an empirical effort because many input parameters cannot be predicted with sufficient accuracy on before hand. Examples of such input parameters are climate, traffic and the quality of the materials as laid and the variation therein. All this means that although advanced methods provide a much better insight in why pavements behave like they do, one should realize that even with the most advanced methods one only can achieve a good estimate of e.g. pavement performance. Obtaining an accurate prediction is still impossible. Because of this, practice is very much interested in design methods which are, on one hand, based on sound theoretical principles but, on the other hand, are very user friendly and require only a limited amount of testing in order to save money and time. One should realize that the need to use accurate modeling is influenced to a very large extent by the type of contracts used for road construction projects. In recipe type contracts, the contractor is only responsible for producing and laying mixtures in the way as prescribed by the client. In this case the contractor is neither responsible for the mixture design nor the design of the pavement structure; these are the responsibilities of the client. This immediately implies that the clients in this case will choose proven designs and materials, in other words he will rely on experience, and the contractor has no incentive to spend much effort and resources in advanced material research and pavement design methods. If however contractors are made more responsible for what they make, meaning that contractors take over from the authorities the responsibility for the performance of the road over a certain period of time, then they are much more willing to use more advanced ways of material testing and pavement design. The purpose of these lecture notes is not to provide an overall picture of existing mechanistic empirical design methods. The goal of these notes is to provide an introduction into pavement design using the analytical methods and material characterization procedures as they are common practice nowadays in the Netherlands. This implies that we will concentrate in these notes on the use of multi layer linear elastic systems and the material characterization needed to

27

use these systems. Also attention will be paid to how to deal with pavement design in case the main body of the structure consists of unbound materials which exhibit a stress dependent behaviour. Also the characterization of lime and cement treated layers will be discussed.

5.2 Stresses in a homogeneous half space Although pavement structures are layered structures, we start with a discussion of the stresses in a homogeneous half space. Solutions for this were first provided by Boussinesq at the end of the 1800s. Originally Boussinesq developed his equations for a point load but later on the equations were extended for circular wheel loads. The stresses under the center of the wheel load can be calculated using: z = p [ -1 + z3 / (a2 + z2)3/2 ] r = t = [ -(1 + 2) + 2.z.(1 + ) / (a2 + z2) { z / (a2 + z2) }3 ] . p / 2 w = 2.p.a.(1 - 2) / E Where: z = vertical stress, r = radial stress, t = tangential stress, = Poissons ratio, E = elastic modulus, a = radius of the loading area, p = contact pressure, z = depth below the surface. Please note that the cylindrical coordinate system is used for the formulation of the stresses (see figure 26). This is not the place to give the derivations that resulted in the equations given above. The interested reader is referred to [4, 6]. In figure 27 some graphical solutions are provided for the Boussinesq equations.

The Boussinesq equations are useful to estimate stresses in e.g. earth roads where the road structure is built by using the natural available material. One can e.g. derive the Mohrs circles from the calculated stresses and then one can determine whether the stresses that occur are close to the Mohr Coulomb failure line, implying early failure, or not. Many of these earth roads however are layered systems simply because the top 200 mm or so have different characteristics than the original material simply because of compaction that is applied etc. The higher stiffness of this top layer results in a better spreading of the load. This is schematically shown in figure 28.

28

Figure 26: Cartesian and cylindrical coordinate system.

29

Figure 27: Graphical solutions for Boussinesqs equations.

30

Figure 28: Effect of applying a stiffer top layer on the spreading of the load. In order to be able to calculate stresses in such two layered systems, Odemarks equivalency theory [13] is of help. The idea behind Odemarks theory is that the vertical stresses at the interface between the top layer with stiffness E1 and thickness h1 and the half space with stiffness Em are the same as the stresses at an equivalent depth heq with stiffness Em. This principle is shown in figure 29.

Figure 29: Principle of Odemarks equivalency theory.

The figure shows on the left hand side the distribution of the vertical stresses in a two layer system. On the right hand side the equivalent heq is shown resulting in the same vertical stress (B) at the interface between the top layer and the underlying half space. Odemark showed that the equivalent layer thickness can be calculated using: heq = n h1 (E1 / Em)0.33

Em Em

h1

A

A

BB E1

Em Em

E1

heq Em

31

If Poissons ratio of the top layer equals Poissons ratio of the half space, then n = 0.9. The question of course is how well this Odemark/Boussinesq approach allows accurate predictions of the vertical stresses in pavements to be made. As is shown in figure 30 [14], this approach seems to be fairly effective in case one is dealing with pavements having unbound bases and subbases.

Figure 30: Comparison of measured and calculated vertical stresses in pavements.

Let us illustrate the procedure by means of an example. We want to know the stresses in a homogeneous half space (modulus 100 MPa) that is loaded with a wheel load of 50 kN. Since the contact pressure is known to be 700 kPa, we can calculate the radius of the loading area following: p a2 = Q Where: p = contact pressure, a = radius of the contact area, Q = wheel load. In this way we calculate a = 150 mm. If we assume Poissons ratio to be 0.25, then we can derive from figure 27 that the vertical stress under the centre of the load at a depth of 150 mm (z = a) is to 60% of p being 420 kPa. Assume that this stress is too high and that a layer is placed on top of the half space having a modulus of 300 MPa and a thickness of 150 mm. The equivalent layer thickness of this layer is:

32

heq = 0.9 h1 (E1 / Em)0.33 = 0.9 * 150 * (300 / 100)0.33 = 194 mm We can now calculate the vertical stress using the same Boussinesq chart but this time the depth at which we have to determine the stress is 194 + 150 = 344 mm which is at a depth of z = 2.3 a. From figure 27 we notice that now the vertical stress is equal to approximately 20% of p being 140 kPa.

5.3 Stresses in two layer systems If the stresses in the subgrade, the half space, due to the wheel load are too high, a stiff top is needed to reduce these stresses. Such a system, a stiffer layer on top of a softer half space, is called a two layer system. It could represent e.g. a full depth asphalt pavement on top of a sand subgrade. Burmister [5] was the first one who provided solutions for stresses in a two layer system. Again, it is beyond the scope of these lecture notes to provide a detailed discussions on the mathema-tical background. Here only attention will be paid to the results of those mathematical analyses and how they can be used in practice. Figure 31 shows the effect of a stiff top layer on the distribution of the vertical stresses in a two layer system. First of all we notice that the distribution of the vertical stress is bell shaped. Furthermore we notice that the magnitude of the vertical stress is quite influenced by the stiffness of the top layer. The width of the stress bell however is much less influenced by the stiffness of the top layer.

Figure 31: Distribution of the vertical stress in a one and two layer system.

A stiff top layer not only provides protection to the second layer, also tensile stresses at the bottom of the top layer develop. These stresses are due to bending of the top layer. This implies that for two layer systems we are dealing with two design parameters being the horizontal tensile

33

stress at the bottom of the top layer and the vertical compressive stress at the top of the second layer (figure 32).

Figure 32: Design criteria in a two layer pavement system.

If the horizontal tensile stress at the bottom of the top layer is too high, it will be the cause for cracking of the top layer. If the vertical compressive stress at the top of the bottom layer is too high, excessive deformation will develop in that layer.

Figure 33 shows the distribution of the horizontal and vertical stresses in a two layer system under the centre of the load in relation to the ratio E1 / E2 and for h = a. Please note that Poissons ratio is 0.25 for both layers.

Figure 33a: Distribution of the horizontal stresses in a two layer system under the centre of a circular load (Poissons ratio equals 0.25).

horizontal tensile stress E2 vertical compressive stress

E1, h1

34

Figure 33b: Distribution of the vertical stresses in a two layer system under the centre of a circular load.

From the figure 33a one can observe that significant horizontal stresses develop in the top layer. When E1 / E2 = 10, a tensile stress equal to the contact pressure p develops while this value becomes 2.7 * p when E1 / E2 = 100. One also observes that at those modulus ratios the tensile stresses in the second layer can almost be neglected. Another interesting aspect is that the neutral axis is almost in the middle of the top layer for modulus ratios of 10 and higher. Figure 33b shows that a stiff top layer greatly reduces the vertical stresses in the bottom layer. As we have seen in figure 27, the stress at a depth of z = a is 60% of the contact pressure in case of a half space. Figure 33b shows that if the modulus ratio is 10, the vertical stress at z = a is only 30% of the contact pressure. Let us go back for a moment to Odemarks equivalency theory. We have noticed that in a half space, the vertical stress at a depth of z = a under the centre of the load equals 60% of the contact pressure. If we assume that the top part of that half space is replaced over a depth of a by a material that has a 10 times higher modulus, than the equivalent layer thickness of that layer equals: heq = 0.9 * a * (10)0.33 = 1.92 * a From figure 27 we can determine that the vertical stress at that depth equals approximately 30% of p. This is in excellent agreement with the result obtained from figure 33b. This is considered to be proof of the validity of Odemarks approach.

35

Until now no attention has been paid to the conditions at the interface. From our structural design classes we know that it makes quite a difference whether layers are perfectly glued to each other and there is no slip (full friction) between the layers or whether the layers can freely move over each without any friction (full slip). The effect of those two interface conditions on the stresses at the bottom of the top layer are shown in figure 34.

Figure 34a: Influence of friction on the radial stresses at the bottom of the top layer under the

wheel centre (please note that Poissons ratio is 0.5).

36

Figure 34b: Influence of friction on the vertical stress at the top of bottom layer under the wheel

centre (please note that Poissons ratio is 0.5).

As one will observe, the presence of friction has a significant influence on the radial (horizontal) stress at the bottom of the top layer especially at low values for the ratio E1 / E2. We also note that the influence on the vertical stress is much smaller. If there is full friction or full bond at the interface, the following conditions are satisfied.

37

a. The vertical stress just below and above the interface are equal because of equilibrium, so: z bottom, top layer = top, bottom layer b. The horizontal displacements just above and below the interface are the same because of full friction, so: ur bottom, top layer = ur top, bottom layer c. The vertical displacements just above and below the interface are the same because of continuity, so: uz bottom, top layer = uz top, bottom layer In case of full slip, only conditions a. and c. are satisfied. Another important factor is Poissons ratio. Since measurements needed to determine Poissons ratio are somewhat complicated, values for this parameter are usually estimated from information available from literature. The question then is to what extent wrong estimates influence the magnitude of the stresses. Information on this can be found in figure 35. Figure 35a e.g. shows that the influence of Poissons ratio on the radial stress at the bottom of the asphalt layer is quite significant. This also means that it will have a significant influence on the radial strain. As one can see from figure 35b, the influence of Poissons ratio on the vertical stress at the top of the bottom layer is limited.

Figure 35a: Influence of Poissons ratio on the radial stress at the bottom of the top layer.

38

Figure 35b: Influence of Poissons ratio on the vertical stress at the top of the bottom layer.

By means of the figures available we now can estimate the stresses and strains in two layer pavements. This will be illustrated by means of the following example. Assume we have a two layer structure consisting of a 150 mm thick asphalt layer on top of a sand subgrade. The elastic modulus of the asphalt layer is 5000 MPa while the modulus of the sand layer is 100 MPa. A 50 kN wheel load is applied on the pavement. The contact pressure 700 kPa which results in a radius of the circular contact area of 150 mm. Poissons ratio for both the asphalt and the sand layer equals 0.35. We want to know the stresses and strains in the locations indicated below.

Figure 36: Two layer pavement example problem.

Let us start with the calculation of the stresses and strains at the bottom of the asphalt layer. Since both layers have a Poisson ratio of 0.35, we have to use figure 35 and interpolate between the lines for = 0.25 and = 0.5. Since E1 / E2 = 50 and a / h = 1 we read from the graphs

Pavement surface, z = 0 Bottom of asphalt layer, z = 150 mm

Top of sand layer, z = 150 mm

Asphalt h = 150 mm E = 5000 MPa = 0.35 Sand E = 100 MPa = 0.35

39

shown in figure 37 that -r / p = 2.7 and z / p = 0.15. Since the contact pressure is a compressive stress and we decided to express compression by means of the minus sign (-), we calculate r = t = 1890 kPa and z = -105 kPa. Please note that under the centre of the load centre there is not only a horizontal radial stress r but also a horizontal tangential stress t (see also figure 26). These stresses are acting perpendicular to each other and because the load centre is in the axis of symmetry, the tangential stress is equal to the radial stress.

Figure 37a: Estimation of the horizontal stress at the bottom of the asphalt layer.

40

Figure 37b: Estimation of the vertical stress at the top of the subgrade.

The strains are calculated as follows: r = t = (r - t - z) / E = (1890 0.35 * 1890 0.35 * -105) / 5000000 = 2.53 * 10-4 z = (z -r - t) / E = (-105 0.35 * 1890 0.35 * 1890) / 5000000 = -2.86 * 10-4 Please note that the units used for the stresses and elastic modulus is kPa. This implies that the value of 5000000 is used for the modulus (originally it was given in MPa). Let us now consider the stresses and strains at the top of the asphalt layer. We notice that figure 35 is not of help anymore because that figure only gives information about the stresses at the bottom of the asphalt layer. We know however that, for reasons of equilibrium, the vertical stress at the top of the asphalt layer is equal to the contact pressure, so z = -700 kPa. There are no graphs available to estimate the horizontal stress at the top of the asphalt layer for = 0.35, but we can make a reasonable estimate of those stresses. From figure 35 we determine that the tensile stress at the bottom of the asphalt layer is -2.2 * p if = 0.25. If we insert that value in figure 33, then we can determine that the radial stress at the top of the pavement equals 2.5 * p (see figure 38).

41

Figure 38: Estimation of the horizontal stress at the top of the asphalt layer. Going back to figure 35a we notice that the radial stresses at the bottom of the asphalt layer are 2.7 * p / 2.2 * p = 1.23 times higher when = 0.35 instead of 0.25. Therefore we estimated the radial compressive stress at the top of the asphalt layer to be 1.27 * 2.5 * p = -2223 kPa (the sign is because p is compressive). Using these values we calculate: r = t = (r - t - z) / E = (-2223 0.35 * -2223 0.35 * -700) / 5000000 = -2.4 * 10-4 z = (z - r - t) / E = (-700 0.35 * -2223 0.35 * -2223) / 5000000 = 1.71 * 10-4 This later value implies that a vertical tensile strain develops at the top of the asphalt layer! Finally we will discuss the stresses and strains at the top of the subgrade. Because of equilibrium, the vertical stress at the top of the subgrade is equal to the vertical stress at the bottom of the asphalt layer being -105 kPa. Also in this case we have no graphs available to estimate the horizontal stresses at the top of the subgrade. Nevertheless figure 33a is showing that the radial stress at the top of the subgrade is very small and almost zero for E1 / E2 = 100. For that reason we assume that at the top of the subgrade r = t = 0. Using these values we calculate: r = t = (r - t - z) / E = (0 0 0.35 * -105) / 100000 = 3.68 * 10-4 z = (z - r - t) / E = (-105 0 0) / 100000 = -1.05 * 10-3

5.4 Stresses in three layer systems The calculation of the stresses and strains in three layer systems is based on the same principles as used for two layer systems. It is however much complicated to derive tables [7] and charts [8] that allow the stresses at various points in the pavement to be estimated and as we will see from the given examples, those charts are not very user friendly. Figure 39 shows the stresses and locations in a three layer system for which tables and graphs have been developed. Note that a Poissons ratio of 0.5 was used for all layers.

42

Figure 39: Locations in a three layer system for which tables and graphs to estimate stresses

have been developed.

In developing those tables and graphs, the following parameters have been used. A = a / h2; H = h1 / h2; K1 = E1 / E2; K2 = E2 / E3 Figures 40, 41 and 42 show the graphs for the estimation of resp. zz1, zz2, and rr1 for K1 =20 and K2 = 2.

Diameter 2a, contact pressure p

z1 r1

z2

E1 , h1 E2 , h2 E3 A = a / h2 K1 = E1 / E2 K2 = E2 / E3 H = h1 / h2

43

Figure 40: Chart to estimate zz1 (vertical stress at the top layer base interface) in a three layer

system.

44

Figure 41: Chart to estimate zz2 (vertical stress at the base subgrade interface) in a three layer

system.

45

Figure 42: Chart to estimate rr1 (horizontal stress at the bottom of the top layer at the top layer

base interface) in a three layer system.

The use of the charts is illustrated by means of an example. Let us assume we have a three layer system consisting of 100 mm of asphalt (E = 6000 MPa) that is placed on a 300 mm thick base (E = 300 MPa) on a subgrade with a stiffness with E = 150 MPa. The magnitude of the load is 50 kN and the radius of the loaded area is 150 mm. This implies that the contact pressure is 700 kPa. This input means that K1 = 20, K2 = 2, A = 2 and H = 0.33. We want to know the horizontal stress at the bottom of the asphalt layer. Using figure 42 in the way as illustrated in figure 43, we derive that the horizontal stress factor is approximately 7 which results in rr1 = 7 * 700 = 4900 kPa.

46

Figure 43: Example of the estimation of rr1.

It is obvious that the determination of the stresses in this way is a quite time consuming approach especially since most of the time interpolations have to be made between the different charts. Furthermore the charts are only valid for Poissons ratio equals 0.5 and most materials have a different value for this parameter. Therefore use of one of the many computer programs that are available nowadays is highly recommended.

47

5.5 Stresses due to horizontal loads It is obvious that in reality not only vertical stresses are applied on the pavement surface. Also horizontal shear stresses are present, acting in the longitudinal and transverse direction. These shear stresses are due to traction forces, braking, cornering etc. They occur under free rolling as well as driven tires. As we will see in the next chapter, the real stress conditions in the contact area are indeed very complex. Several researchers have studied the effect of such shear forces and early work on this topic is done by Verstraeten [15] and Wardle and Gerrard [16]. Given the limited computational power in those days, they had to apply rigorous simplifications of the real stress conditions. Nevertheless, a good idea of the effect of these shear stresses can be obtained from their work. Figures 44, 45 and 46 are taken from the work presented by Verstraeten. The figures show that depending on the applied shear force, significant radial and tangential stresses can develop at the pavement surface. Furthermore the figures show that the ratio of stiffness of the top layer over the stiffness of the second layer has a large effect on the magnitude of these stresses. It will be obvious that the ratios h1/a and h2/h1 will have a significant effect on the stresses at the interface.

48

Figure 44: Radial and tangential stresses in a pavement system due to a uniformly distributed,

unidirectional, shear load.

49

Figure 45: Vertical stresses in a pavement system due to a uniformly distributed, unidirectional

shear load.

50

Figure 46: Radial stresses in a pavement system due to a combination of vertical stresses and

uniformly distributed, unidirectional and multidirectional, shear forces.

51

5.6 Stresses in multilayer systems, available computer programs As has been mentioned in the previous section, it is strongly recommended to use a multilayer computer program for the analysis of stresses and strains in three layer systems. This becomes a necessity in case the number of layers is 4 or more. Charts for the assessment of stresses in a four layer systems even dont exist. Many computer programs have been developed in time and it is almost impossible to give a complete picture of the available programs. Well known programs are BISAR, KENLAYER, CIRCLY, and WESLEA. BISAR and WESLEA only allow linear elastic materials to be taken into account. CIRCLY on the other hand allows taking into account anisotropic behavior of materials. Many of these programs have been incorporated in design systems such as the Shell Pavement Design System, CARE (developed in the Netherlands), mePADS (developed in South Africa). KENLAYER is an interesting system because it allows taking into account the stress dependent behaviour of unbound granular materials and soils. RUBICON, a program developed in South Africa, is a finite element based program that also allows to take into account the stress dependent behavior of granular materials. Furthermore this program allows probabilistic analyses to be made. Many of these programs can be found on the internet and can be retrieved for free while other software packages (mainly the design systems) have to be purchased. It is beyond the scope of these lecture notes to discuss all the available programs in detail. In this part of the lecture notes we only discuss the output that is generated by computer programs that just calculate the stresses and strains in the pavement system due to traffic loads. In order to do so we will use the output as provided by BISAR developed by Shell. First of all however attention is paid to the quality of such programs. It is generally accepted that the BISAR program can be taken as the reference to which all other programs can be compared. This is because of the high mathematical stability of the BISAR program. Quite some programs have minor flaws of which the user should be aware before using them. To check whether these flaws exist the stresses, strains and displacements have to be calculated in a number of points of the pavement structure (see figure 47).

Figure 47: Locations in the pavement where consistency checks can be made.

Is v equal to contact pressure?

Is the vertical displacement cq vertical stress cq horizontal displacement at the top of layer 2 at z = h1 equal to the vertical displacement cq vertical stress cq horizontal displacement at the bottom of layer 1 at z = h1?

Are realistic values obtained for the stresses and strains at the edge of the load?

Is the vertical displacement cq vertical stress cq horizontal displacement at the bottom of layer 2 at z = h1 + h2 equal to the vertical displacement cq vertical stress cq horizontal displacement at top of layer 3 at z = h1 + h2

Full bond between the layers is assumed

52

Some programs do not fulfill the requirements set for the interface between layers 1 and 2 or the interfaces between layers 2 and 3. These programs often also not fulfill the equilibrium requirement at the pavement surface under the centre of the load. More programs generate unrealistic results at the edge of the load. The problems at the interfaces and under the centre of the load at the pavement surface can easily be overcome by not requiring output at those interfaces but at locations that are e.g. 1 mm above or below the interface. Almost all programs generate comparable results if stresses and strains are required at other locations in the pavement. Although most of the problems mentioned above can be overcome quite easily, one must be aware of the fact that some programs have difficulties in generating realistic results for pavements with a thin asphalt layer that has a low modulus on top on a thick stiff (high modulus) base layer (so if h1 / h2 < 1 and E1 / E2 < 1). It should be noted that the BISAR program passes all these requirements. Let us now return to the output that is generated by these computer programs and let us explain the output that is generated by BISAR for two example problems. The two problems that are analyzed are schematically shown in figure 48.

Figure 48a: Example problem.

Figure 48b: Coordinate system and direction of the shear force as used in the example problem.

Fvertical = 50 kN Fhorizontal = 20 kN diameter loaded area = 300 mm

E1 = 6000 MPa h1 = 250 mm 1 = 0.35

E2 = 100 MPa 1 = 0.35

x

y

53

In the first example, only the vertical load is applied while in the second example the vertical and horizontal load is applied. The horizontal load acts in the x-direction and simulates a braking force. The stresses and strains are requested at the following x, y and z coordinates. Load Sheet Layer X [mm] y [mm] z [mm] Vertical force only 2 1 0 0 0 3 1 152 0 0 4 1 152 0 10 5 1 0 0 250 6 2 0 0 250 Vertical and 8 1 -152 0 0 horizontal force 9 1 0 0 0 10 1 152 0 0 11 1 -152 0 10 12 1 0 0 10 13 1 152 0 10 14 1 0 0 250 15 2 0 0 250

Table 5: Locations where results are obtained. Note: The sheet number refers to the handwritten numbers written on the output pages given in figure 49.

Please note that at the pavement surface and at a depth of 10 mm, the results are requested just outside the loaded area and at the load centre. This is done to determine the effect of the shear forces. In figure 49 all the calculation results are given while the main results are summarized in table 6. Sheet nr. 1 [Pa] 2 [Pa] 3 [Pa] 1 2 3 2 -7.074E+05 -1.251E+06 -1.251E-6 2.800E-05 -9.421E-05 -9.241E-053 0 -4.231E+05 -6.758E+05 6.410E-05 -3.110E-05 -8.975E-054 -1.630E+05 -7.555E+05 -8.132E+05 6.434E-05 -6.897E-05 -8.195E-055 9.046E+05 9.046E+05 -3.547E+04 1.001E-04 1.001E-04 -1.115E-046 -3.705E+03 -3.705E+03 -3.547E+04 1.001E-04 1.001E-04 -3.288E-048 4.618E+05 0 -4.179E+05 1.013E-04 -2.565E-06 -9.658E-059 -5.867E+05 -1.251E+06 1.371E+06 5.514E-05 -9.421E-05 -1.213E-0410 0 -9.337E+05 -1.308E+06 1.308E-04 -7.932E-05 -1.635E-0411 -9.085E+04 -2.962E+05 -6.034E+05 3.733E-05 -8.874E-06 -7.798E-0512 -5.887E+05 -1.122E+06 -1.239E+06 3.985E-05 -8.034E-05 -1.067E-0413 -2.154E+05 -9.076E+05 -1.350E+06 9.578E-05 -5.996E-05 -1.595E-0414 9.046E+05 9.046E+05 -3.547E+04 1.001E-04 1.001E-04 -1.115E-0415 -3.694E+03 -3.705E+03 -3.548E+04 1.002E-04 1.002E-04 -3.289E-04

Table 6: Results of the example problems in terms of principal stresses and strains. On sheets nr 1 and nr 7 of figure 49, we recognize the input. Please note on sheet 7 that the angle of the shear load is taken from the x-axis. Since the horizontal load is acting in the positive x-direction the shear direction equals 00 (the angle equals 1800 if the shear load is acting in the negative x-direction). If the shear force was acting in the positive y-direction, the shear direction had to be 900. The sheets with the calculation results are pretty much self explaining. The coordinates of the location at which the stresses and strains are requested are given in the top of

54

Figure 49a: Input for BISAR calculation; vertical load only.

55

Figure 49b: Output of BISAR calculation.

56

Figure 49 c: Output of BISAR calculation (continued).

57

Figure 49d: Output of BISAR calculation (continued).

58

Figure 49e: Output of BISAR calculation (continued).

59

Figure 49f: Output of BISAR calculation (continued).

60

Figure 49g: Input for BISAR calculation; vertical and shear load.

61

Figure 49h: Output of BISAR calculation.

62

Figure 49i: Output of BISAR calculation (continued).

63

Figure 49j: Output of BISAR calculation (continued).

64

Figure 49k: Output of BISAR calculation (continued).

65

Figure 49l: Output of BISAR calculation (continued).

66

Figure 49m: Output of BISAR calculation (continued).

67

Figure 49n: Output of BISAR calculation (continued).

68

Figure 49o: Output of BISAR calculation (continued).

69

the page. Then detailed information is given on the normal stresses and strains acting in the XX, YY and ZZ direction as well as on the shear stresses and strains in the YZ, XZ, and XY direction. All this information is summarized in terms of principal stresses and strains as well as the directions in which these principal stresses and strains are acting. In table 6 a summary is given of these principal stresses and strains. When the results of sheet 5 (vertical load, bottom of the asphalt layer) are compared with those of sheet 14 (vertical load + shear load, bottom of the asphalt layer), we observe that those are exactly the same. This implies that the effect of the shear force is not visible at a depth of 250 mm. The same is true if we compare the results of sheets 6 and 15. The effect of the shear force is clearly visible when the results of sheet 3 (vertical load, location just outside loaded area at pavement surface) are compared with those obtained of sheets 8 and 9 (vertical load + shear load, location just outside loaded area at pavement surface). In case of only a vertical load, xx = -0.423 MPa (sheet 3). In case of a vertical and a horizontal load xx = -1.308 MPa (sheet 10) or xx = 0.462 MPa (sheet 8). As one will observe, the applied braking force results in significant compressive horizontal stresses in front of the load in the direction of travel (x-direction) and a significant tensile stress at the back of the load. The principal strain at the pavement surface just behind the braking load (sheet 8) is slightly larger than the principal strain at the bottom of the asphalt layer (both are acting in the XX direction). Comparison of the results given in sheet 8 with those given in sheet 11 and comparison of the results given in sheet 10 with those given in sheet 13 show how the stresses and strains decrease with depth. From this analysis it becomes clear that proper modeling of the contact stresses is very important in order to be able to analyze surface defects.

6. Axle loads, wheel loads and contact pressures 6.1 Axle loads In order to be able to design a pavement structure, knowledge on the magnitude of the traffic loads is essential. Axle load measurements are therefore made to determine the number and weight of the axles passing over the pavement. Axle load measurements can be made in different ways varying between the up to date system shown in figure 50, to the much more simple system shown in figure 51. The system as shown in figure 50 uses piezoelectric and coax cables to measure the axle load and other features of the truck. Such features include the speed of the truck as well as its registration number. Other items are the distance between the axles, the total length of the vehicle and a classification is made of the type of truck. This example shows amongst other things that the heaviest axle load is the tandem axle of the truck. The second axle from the front end of the truck was carrying a load of 223 kN (22.3 tons) while the third axle from the front carried 210 kN (21 tons). Comparing these values with the axle load regulations that prevail in the Netherlands (table 7), shows that the tandem axle is severely overloaded.

70

Figure 50: Example of a modern axle load survey unit as used in the Netherlands.

Maximum axle load driven axles (no restrictions with respect to suspension system, tires and steering)

115 kN

Maximum axle load non driven axles 100 kN Maximum axle load tandem axles Axle distance < 1.0 m 1.0 m axle distance < 1.3 m 1.3 m axle distance < 1.8 m without air suspension system 1.3 m axle distance < 1.8 m with air suspension system

100 kN 160 kN 180 kN 190 kN

Maximum axle load triple axles Axle distance < 1.3 m 1.3 m axle distance < 1.8 m without air suspension system 1.3 m axle distance < 1.8 m with air suspension system

210 kN 240 kN 270 kN

Table 7: Axle load regulations in the Netherlands.

71

Figure 51 shows the axle load unit that was used in Ghana during an axle load survey program sponsored by the European Union [17]. The unit consisted of 4 Haenni WL 103 scales which were arranged in such a way that first the outer wheel of an axle were weighed and after that the total axle weight. This measurement procedure allowed to determine whether or not all the wheels of an axle were carrying the same load. Table 8 shows the axle load distributions as they are used in the Netherlands as input for the thickness design of concrete pavements [18].

Table 8: Axle load distributions as used in the Netherlands for the design of concrete pavements. Table 8 is also suggested for use for the design of flexible pavements. Table 9 shows the results of the axle load survey in Ghana as reported in [17].

Axle load frequency distribution (%) for different types of road Axle loadgroup (kN)

Average wheel load P (kN)

heavily loaded motorway

normally loaded motorway

heavily loaded pro-vincial road

normally loaded pro-vincial road

municipal main road

rural road

public transport bus lane

20-40 15 20.16 14.84 26.62 24.84 8.67 49.38 - 40-60 25 30.56 29.54 32.22 32.45 40.71 25.97 - 60-80 35 26.06 30.22 18.92 21.36 25.97 13.66 - 80-100 45 12.54 13.49 9.46 11.12 13.66 8.05 - 100-120 55 6.51 7.91 6.50 6.48 8.05 2.18 100 120-140 65 2.71 3.31 4.29 2.70 2.18 0.38 - 140-160 75 1.00 0.59 1.64 0.83 0.38 0.38 - 160-180 85 0.31 0.09 0.26 0.19 0.38 0.00 - 180-200 95 0.12 0.01 0.06 0.03 0.00 0.00 - 200-220 105 0.03 0.01 0.03 0.00 0.00 0.00 - Av. nr. of axles per heavy vehicle

3.5 3.5 3.5 3.5 3.5 3.1 2.5

Figure 51: Simple axle load unit as used for surveys in Ghana

72

Axle load Axle 1 Axle 2 Axle 3 Axle 4 Axle 5 Axle 6 10 1 0 0 0 0 0 20 5 0 0 0 0 0 30 42 3 3 1 0 0 40 110 8 8 7 3 0 50 144 11 13 12 4 0 60 222 33 39 23 4 0 70 123 56 40 27 4 0 80 80 77 63 44 5 0 90 35 68 78 32 4 0

100 21 81 70 48 3 0 110 4 81 49 30 4 0 120 0 86 59 28 9 1 130 0 57 24 19 0 0 140 0 46 39 25 7 0 150 0 41 14 19 4 1 160 0 39 6 4 1 0 170 0 41 5 2 1 0 180 0 28 2 2 2 0 190 0 13 1 5 2 0 200 0 9 0 0 2 0 210 0 5 0 0 0 0 220 0 2 0 0 0 0 230 0 2 0 0 0 0 240 0 1 0 0 0 0

axle load summary [kN] max 112,5 236,5 189,0 191,5 203,5 153,5 avg 59,97 116,08 99,08 101,25 108,96 135,5 sa 16,77 38,06 28,43 31,75 43,10 25,46 tire pressure [kPa] max 1050 1015 980 980 945 840 avg 756 798 805 819 826 840 sa 105 77 63 56 49 0

Table 9: Results of axle load surveys in Ghana.

The results were obtained by means of axle load surveys carried out in Ghana on different roads. In total 787 trucks were surveyed. The trucks had either 2, 3, 4, 5 or 6 axles. The axle loads, including the number 1 steering axle, are reported in table 9. The table also shows the maximum axle load measured, as well as the average axle load and the standard deviation. Given the fact that the allowable was 100 kN, it is quite clear that severe overloading occured. This however, is a problem in many countries. The table also shows interesting information with respect to the tire pressures. Normally tires as surveyed should operate at an inflation pressure of around 700 kPa. The table shows that the mean tire pressure was indeed close to this value but also that some very exotic values occurred. These high tire pressures certainly result in high contact stresses and in accelerated pavement damage. Table 10 shows results of axle load measurements as performed in Yemen. Again one notices the large amount of very heavy, overloaded, vehicles.

73

Vehicle type Axle Axle load range [kN] Min. Max. Average Heavy busses 1 30 58 46 (1%) 2 49 107 84 vehicle weight 82 164 130 2 axle medium 1 33 63 47 truck (34%) 2 75 144 115 vehicle weight 115 191 162 2 axle heavy 1 33 99 70 truck (30%) 2 98 243 170 vehicle weight 145 343 240 3 axle truck 1 42 109 74 (30%) 2 67 226 153 3 76 240 161 vehicle weight 187 553 388 4 axle truck 1 45 79 60 (3%) 2 80 202 134 3 80 180 133 4 92 193 136 vehicle weight 227 595 395 5 axle truck 1 44 89 67 (2%) 2 52 161 110 3 52 169 109 4 68 204 142 5 70 201 151 vehicle weight 327 736 577

Table 10: Axle loads for the Hodeidah Sanaa road [19]. Note: the percentages given are the percentages of occurring.

Table 11 is another example of overloading conditions. The results presented in that table are from axle load surveys done on the Jing-Zhu freeway in the Hubei province, China [20]. The table not only shows a significant amount of overloading (legal load limit is 100 kN) but also clearly indicates that the overload problem rapidly increased during the 1995 1998 period. From the information given so far, it is clear that an as good as possible estimation of the axle load distribution is essential. Overloading seems to be a problem in many countries and one should realize that especially the heavy, overloaded vehicles are causing most of the pavement damage. At this moment it is appropriate to recall the concept of load equivalency. This concept implies that one determines the damaging effect of a particular axle load relative to a standard axle load. The equivalent number of load repetitions is calculated using:

Neq = (L/Lref)m NL

Where: Neq = number of equivalent passages of the axle load considered, L = axle load to be considered,

Lref = reference axle load, NL = number of repetitions of the axle passages considered, m = damage factor.

74

The equation implies that if the reference axle equals 100 kN and assuming m = 4, a 200 kN axle produces 16 times more damage than the reference axle does. It should be noted that the value of m depends on which damage type is considered. If one wants to know the damaging effect of various axle loads relative to each other in terms of fatigue of the asphalt layer, then 3 < m < 6. If the effect on fatigue in a cement treated layer has to be considered, then 7 < m < 10. If the effect on the loss of serviceability needs to be considered then m = 4.

Table 10: Axle loads on the Jing-Zhu freeway in China.

6.2 Wheel loads One would expect that the wheel load is equal to the axle load divided by the number of wheels on the axle. This however is not true. Figure 52 e.g. shows that chamber of the pavement surface results in an unequal sharing of the axle load over both wheel groups of the axle.

Figure 52: Chamber of the roads results in unequal sharing.

`` The wheel group on the verge side of the road carries 52% of the load while the wheel group near the centre line of the road carries 47%. Wheel load measurements as carried out in Ghana [17] showed however that quite often the axle load was far from equally distributed over the wheels of the axle; some examples are shown in figure 53.

Axle load (kN)

< 60 60-100 100-130 130-150 150-180 >180 total

Year

no. % no. % no. % no. % no. % no. % no. %

1995 893 25.86 811 23.49 811 23.49 420 12.16 352 10.19 166 4.81 3453 100

1996 899 20.26 1027 23.15 1026 23.14 665 14.99 557 12.55 263 5.93 4437 100

1997 981 18.74 1218 23.26 1217 23.24 815 15.57 682 13.02 322 6.15 5235 100

1998 1078 17.66 1193 19.54 1192 19.52 1183 19.38 991 16.23 468 7.67 6105 100

75

Figure 53: Examples of unequal sharing of the axle load over the wheels.

6.3 Contact pressures As mentioned before, knowledge on axle and wheel loads is important but even more so is knowledge on the contact pressures. Wheel loads come in different sizes and shapes, some of them are shown in figure 54, and each of them produces a different contact pressure distribution.

76

Figure 54: Different tire types.

The well known dual tire configuration is shown on the left of figure 54; it is used all over the world for the driven and towed axles. Normally these tires have an inflation pressure of around 700 kPa. The steering axle of a truck always has a single tire, having the same dimensions as one of the dual tires. In western Europe however, most of the towed axles are equipped nowadays with a so called wide base or super single tire. This tire is shown on the far right of the picture. Normally the tire has an inflation pressure of 800 850 kPa. Next to the super single tire, the super super single tire is shown. This tire is still under development but will be used under the driven axle of trucks thereby replacing the dual wheel configuration. In between the super super single and the dual wheel is a small size dual wheel. This tire is not very much used yet. The idea behind it was that a smaller size tire would allow lowering the loading platform re